Exciton properties in zincblende InGaN-GaN quantum wells under the effects of intense laser fields
© Duque et al.; licensee Springer. 2012
Received: 18 July 2012
Accepted: 18 August 2012
Published: 31 August 2012
In this work, we study the exciton states in a zincblende InGaN/GaN quantum well using a variational technique. The system is considered under the action of intense laser fields with the incorporation of a direct current electric field as an additional external probe. The effects of these external influences as well as of the changes in the geometry of the heterostructure on the exciton binding energy are discussed in detail.
KeywordsNitrides Excitons Intense laser field Quantum wells
InGaN-based systems have revealed a high prospect for applications in optoelectronics. Although the hexagonal (wurtzite) allotropic form is the one most commonly considered, the zincblende (ZB) III-V nitrides are also very promising materials that have been obtained with high-quality crystal structure[1–4]. This is mostly due to the fact that the cubic symmetry avoids the presence of rather high spontaneous polarizations in the crystal, which are, in a greater extent, responsible for the presence of large built-in fields in wurtzite-based heterostructures, responsible for important reductions in the oscillator strength, and the optical recombination rates in that kind of systems[5, 6]. However, the ZB structure in nitrides is provided with higher carrier mobilities, larger optical gain and lower threshold current density because of its smaller effective mass, and has mirror facets compatible with substrates such as GaAs[7–9]. In consequence, the ZB nitride-based heterostructures have drawn much attention in recent times[10–13].
The knowledge of exciton states is important for the correct understanding of some optical properties in the semiconducting low-dimensional systems. Investigations on excitons and related optical properties in ZB nitride low-dimensional systems have been mostly performed in quantum dots[14–18], but much less in quantum well (QW) heterostructures[19, 20].
Research activities on the interaction of intense laser fields (ILF) with carriers in semiconductor nanostructures have revealed interesting physical phenomena. For instance, the presence of changes in the electron density of states in QWs and quantum well wires (QWWs)[21, 22], the measurement of zero-resistance states in two-dimensional electron gases under microwave radiation, terahertz resonant absorption in QWs, and Floquet-Bloch states in single-walled carbon nanotubes, among others. A number of investigations on the effect of laser fields on low dimensional heterostructures have been published. The dressed atom approach was extended by Brandi et al.[26, 27] to treat the influence of the laser field upon a semiconductor system. In the model, the interaction with the laser is taken into account through the renormalization of the semiconductor effective mass. The appearance of an unexpected transition from single to double QW potential induced by ILF was revealed in a theoretical study from Lima et al.. Within the laser-dressed potential model, it is found that the formation of a double-well potential for values of the laser frequencies and intensities such that the so-called laser-dressing parameter α0 is larger than L/2, where L is the QW width. This fact is associated with the possibility of generating resonant states into the system’s channel as well as of controlling the population inversion in QW lasers operating in the optical pumping scheme.
The present work is concerned with the theoretical study of the effects of ILF on exciton states in single ZB nitride QWs of the InGaN-GaN prototype. The research is extended to include the additional influence of an applied direct (dc) electric field oriented along the growth direction of the system. The paper is organized as follows. In the ‘Theoretical framework’ subsection in the ‘Methods’ section, we describe the theoretical framework. The ‘Results and discussion’ section is dedicated to the results and discussion, and finally, our conclusions are given in the ‘Conclusions’ section.
The electron and hole effective masses and the static dielectric constant have been considered to have the same value (the one in In x Ga1−xN) throughout the In x Ga1−xN-GaN QW.
The method for the obtention of the electron and hole states is based on the work by Xia and Fan.
In Equation 7, I and ω are, respectively, the average intensity and the frequency of the laser, c is the velocity of the light, and A 0 is the amplitude of the vector potential associated with the incident radiation. A detailed discussion on the derivation of 〈V〉(z i α0i) is provided in other studies[28, 33–37].
wherez eh = z e −z h andα 0 = (e A0)/(μ c ω).
where λ is the variational parameter. Besides, and with.
whereE0 is the eigenvalue of the Hamiltonian in Equation 4 without the Coulomb interaction term—the last one at the right hand side—andλmin is the value of the variational parameter in which the energy in Equation 11 reaches its minimum.
Results and discussion
Zincblende III-V nitride heterostructures are strained ones, given the lattice mismatch between the constituent materials. Although we are considering here a (001)-oriented In0.2Ga0.8N-GaN QW configuration, the small indium content does not prevent from taking strain effects into account. In particular, there is a breaking of the degeneracy of heavy and light hole valence bands at the center of the two-dimensional Brillouin zone. In this work, we are including strain effects in the most simple way, that is, by incorporating the strain-induced shifts of the conduction and valence band edges in the unperturbed potential profile configuration for both electrons and holes (see, for instance,[40, 41]). Data related with material properties and confining potential are taken from another work.
Considering the strain effects between the well and barrier materials, the electron and hole confinement potential have been obtained, respectively, by the following:
The effective mass parameters used in the calculations
In the fifth row (Figure1e), the evolution of the confined electron and hole levels as functions ofα0 clearly show the growth in the energy values that resulted from the laser-induced deformation of the conduction and valence band potential profiles. Such modification in the QW shape involves a significant rise of the well bottom which acts by pushing up the energy levels. In the valence band, the original depth of the QW is only enough to accommodate a single heavy-hole level and, according to the basic properties of the confined one-dimensional motion, there will always be one energy level in the hole subsystem. In the conduction band, for sufficiently large laser field intensities, the first excited state is expelled from the QW, and there only remains a single confined level (the ground state one).
The configuration chosen includes an applied laser field with intensity given, in each case, by the parameterα0 = 3L/4. It is seen that for the two lowest values of the well width,E b is a slight decreasing function of F until a certain critical value,F c , of the dc field strength at which initiates an abrupt fall that leads to a constant, limit value, that remains for the rest of the increasing range of the amplitude F. The decrease occurring while F < F c is justified along the same arguments expressed above with regard to the progressive enlargement of the inter-carrier average distance that associates with the loss in electron and hole confinement. The abrupt descent inE b has to do with the escape of one (electron or hole) of the wave functions away from the QW region, towards the infinite barrier on the side it was pushed to by the electric field. The value of the expected electron-hole distance then suffers a sudden rise which reflects in the drop ofE b observed. Augmenting further the dc field strength will function to cause the same effect on the other wave function in such a way that the increase in F will not have any other influence on the polarization because the carriers will remain confined by the infinite barriers at ±L ∞ /2. Therefore, one may see thatE b adopts a constant value when F becomes large enough.
It is worth mentioning that, for all the values of L taken into account, settingα0 = 3L/4implies a great modification of the confining potential profile which, as one of the main features, presents a significantly reduced effective well depth. At the same time, the effect of confinement reduction on the carrier wave functions is more pronounced for narrower QWs, for the allowed energy levels are, initially, placed at higher energy positions. Thus, the application of the not so intense dc fields readily leads to the mentioned wave function escape. This explains why the phenomenon of abrupt change inE b is manifested for smaller dc field intensities.
The curves that correspond to the two highest values of L in Figure5 show an increasing behavior for the smallest electric field amplitudes. This fact relates with the reduction in 〈ϕ|z e −z h |ϕ〉 obtained as a result of the combination of the laser and dc fields on the confinement of the carriers. A small F associates with a slight linear deformation of the already modified (by the laser effect) potential profile. The electron and hole densities of probability are pushed in opposite directions, but the potential well barriers, not so deformed, repel them away. This has the consequence of bringing the two particles a little bit closer and, therefore, of augmenting the strength of their Coulombic interaction. However, when the dc field is augmented, the dominant influence is that causing the spatial spreading of the carrier wave functions, which leads to the decrease inE b . Notice that the pronounced fall is also present when L = 150Å, but for L = 200ÅE b is a rather smooth monotonically decreasing function of F, without any abrupt change. This is because the QW width is large enough to avoid the sudden escape of the wave functions and also because the limiting infinite barriers are much closer to the inner well ones.
The properties of heavy-hole excitons in InGaN-GaN-based quantum wells under intense laser and applied dc electric fields are studied for a set of different values of the fields intensities and the well spatial dimensions. In general, for a fixed geometry of the unperturbed system, the exciton binding energy is a decreasing function of the intense laser field parameter and of the dc electric field, although certain combinations of the two applied field intensities may lead to a rather insensitive behavior of the binding energy with respect to the application of a dc field. It is shown that the changes of the degree of carrier confinement and of the carrier polarization associated to the influence of the laser and the dc fields are mainly responsible for the exciton properties mentioned. To our knowledge, there seem to be no previous reports on exciton properties in zincblende nitride QW induced by intense laser fields. Thus, the results of the present work might be considered as a first approximation to the subject in this kind of systems.
Carlos A Duque is grateful to the Colombian Agencies CODI-Universidad de Antioquia (project: E01535-Efectos de la presión hidrostática y de los campos eléctrico y magnético sobre las propiedades ópticas no lineales de puntos, hilos y anillos cuánticos de GaAs-(Ga,Al)As y Si/SiO2) and Facultad de Ciencias Exactas y Naturales-Universidad de Antioquia (CAD-exclusive dedication project 2012-2013). Miguel E Mora-Ramos thanks Mexican CONACYT for the support through 2011-2012 sabbatical grant no. 180636 and research grant CB-2008-101777. He is also grateful to the Escuela de Ingeniería de Antioquia and the Universidad de Antioquia for hospitality in his sabbatical stay.
- Mizuta M, Fujieda S, Matsumoto Y, Kawamara T: Low temperature growth of GaN and AlN on GaAs utilizing metalorganics and hydrazine. Jpn J Appl Phys 1986, 25: L945. 10.1143/JJAP.25.L945View ArticleGoogle Scholar
- Yoshida S: Growth of cubic III-nitride semiconductors for electronics and optoelectronics application. Physica E 2000, 7: 907. 10.1016/S1386-9477(00)00086-2View ArticleGoogle Scholar
- Hsiao CL, Liu TW, Wu CT, Hsu HC, Hsu GM, Chen LC, Shiao WY, Yang CC, Gällström A, Holtz P-O, Chen CC, Chen KH: High-phase-purity zinc-blende InN on r-plane sapphire substrate with controlled nitridation pretreatment. Appl Phys Lett 2008, 92: 111914. 10.1063/1.2898214View ArticleGoogle Scholar
- Novikov SV, Stanton NM, Campion RP, Morris RD, Green HL, Foxon CT, Kent AJ: Growth and characterization of free-standing zinc-blende (cubic) GaN layers and substrates. Semicond Sci Technol 2008, 23: 015018. 10.1088/0268-1242/23/1/015018View ArticleGoogle Scholar
- Andreev AD, O’Reilly EP: Theory of the electronic structure of GaN/AlN hexagonal quantum dots. Phys Rev B 2000, 62: 15851. 10.1103/PhysRevB.62.15851View ArticleGoogle Scholar
- Schulz S, Schumacher S, Czycholl G: Tight-binding model for semiconductor quantum dots with a wurtzite crystal structure: from one-particle properties to Coulomb correlations and optical spectra. Phys Rev B 2006, 73: 245327.View ArticleGoogle Scholar
- Park SH, Chuang SL: Comparison of zinc-blende and wurtzite GaN semiconductors with spontaneous polarization and piezoelectric field effects. J Appl Phys 2000, 87: 353. 10.1063/1.371915View ArticleGoogle Scholar
- Lagarde D, Balocchi A, Carre H, Renucci P, Amand T, Maries X, Founta S, Mariettem H: Room-temperature optical orientation of the exciton spin in cubic GaN/AlN quantum dots. Phys Rev B 2008, 77: 041304.View ArticleGoogle Scholar
- Marquardt O, Mourad D, Schulz S, Hickel T, Czycholl G, Neugeauer J: Comparison of atomistic and continuum theoretical approaches to determine electronic properties of GaN/AlN quantum dots. Phys Rev B 2008, 78: 235302.View ArticleGoogle Scholar
- Lemos V, Silveira E, Leite JR, Tabata A, Trentin R, Scolfaro LMR, Frey T, As DJ, Schikora D, Lischka K: Evidence for phase-separated quantum dots in cubic InGaN layers from resonant Raman scattering. Phys Rev Lett 2000, 84: 3666. 10.1103/PhysRevLett.84.3666View ArticleGoogle Scholar
- Li SF, Schörmann J, Jas DA, Lischka K: Room temperature green light emission from nonpolar cubic InGaN/GaN multi-quantum-wells. Appl Phys Lett 2007, 90: 071903. 10.1063/1.2475564View ArticleGoogle Scholar
- Husberg O, Khartchenko A, As DJ, Vogelsang H, Frey T, Schikora D, Lischka K, Noriega OC, Tabata A, Leite JR: Photoluminescence from quantum dots in cubic GaN/InGaN/GaN double heterostructures. Appl Phys Lett 2001, 79: 1243. 10.1063/1.1396314View ArticleGoogle Scholar
- Zhu JL, Yang N, Li BL: Exciton spectra and polarization fields modified by quantum-dot confinements. Phys Rev B 2009, 80: 075306.View ArticleGoogle Scholar
- Xia CX, Wei SY: Quantum size effect on excitons in zinc-blende GaN/AlN quantum dot. Micro J 2006, 37: 1408.Google Scholar
- Schulz S, Mourad D, Czycholl G: Multiband description of the optical properties of zincblende nitride quantum dots. Phys Rev B 2009, 80: 165405.View ArticleGoogle Scholar
- Xia CX, Zeng ZP, Wei SY: Effects of applied electric field and hydrostatic pressure on donor impurity states in cylindrical GaN/AlN quantum dot. J Appl Phys 2009, 107: 014305.View ArticleGoogle Scholar
- Xia CX, Zeng ZP, Liu ZS, Wei SY: Exciton states in zinc-blende GaN/AlGaN quantum dot: effects of electric field and hydrostatic pressure. Physica B 2706, 405: 2010.Google Scholar
- Shi L, Yan ZE: Exciton in a strained (001)-oriented zinc-blende GaN/AlxGa1−xN ellipsoidal finite-potential quantum dot under hydrostatic pressure. Phys Stat Sol C 2011, 8: 42. 10.1002/pssc.201000625View ArticleGoogle Scholar
- Chichibu SF, Azuhata T, Okumura H, Tackeuchi A, Sota T, Mukai T: Localized exciton dynamics in InGaN quantum well structures. Appl Surf Sci 2002, 190: 330. 10.1016/S0169-4332(01)00907-2View ArticleGoogle Scholar
- Park SH, Ahn D, Lee YT, Chuang SL: Exciton binding energies in zincblende GaN/AlGaN quantum wells. Japn J Appl Phys 2004, 43: 140. 10.1143/JJAP.43.140View ArticleGoogle Scholar
- Jauho AP, Johnsen K: Dynamical Franz-Keldysh effect. Phys Rev Lett 1996, 76: 4576. 10.1103/PhysRevLett.76.4576View ArticleGoogle Scholar
- Enders BG, Lima FMS, Nunes OAC, Fonseca ALA, Agrello DA, Fanyao Q, Da Silva Jr. EF, Freire VN: Electronic properties of a quasi-two-dimensional electron gas in semiconductor quantum wells under intense laser fields. Phys Rev B 2004, 70: 035307.View ArticleGoogle Scholar
- Mani RG, Smet JH, von Klitzing K, Narayanamurti V, Johnson WB, Umansky V: Zero-resistance states induced by electromagnetic-wave excitation in GaAs/AlGaAs heterostructures. Nature 2002, 420: 646. 10.1038/nature01277View ArticleGoogle Scholar
- Asmar NG, Markelz AG, Gwinn EG, Cerne J, Sherwin MS, Campman KL, Hopkins PF, Gossard AC: Resonant-energy relaxation of terahertz-driven two-dimensional electron gases. Phys Rev B 1995, 51: 18041. 10.1103/PhysRevB.51.18041View ArticleGoogle Scholar
- Hsu H, Reichl LE: Floquet-Bloch states, quasienergy bands, and high-order harmonic generation for single-walled carbon nanotubes under intense laser fields. Phys Rev B 2006, 74: 115406.View ArticleGoogle Scholar
- Brandi HS, Latgé A, Oliveira LE: Interaction of a laser field with a semiconductor system: application to shallow-impurity levels of quantum wells. Phys Stat Sol B 1998, 210(b):671.View ArticleGoogle Scholar
- Brandi HS, Latgé A, Oliveira LE: Laser effects on donor states in low-dimensional semiconductor heterostructures. Phys Rev B 2004, 70: 153303.View ArticleGoogle Scholar
- Lima FMS, Amato MA, Nunes OAC, Fonseca ALA, Enders BG, da Silva Jr EF: Unexpected transition from single to double quantum well potential induced by intense laser fields in a semiconductor quantum well. J Appl Phys 2009, 105: 123111. 10.1063/1.3153963View ArticleGoogle Scholar
- Xia J-B, Fan W-J: Electronic structures of superlattices under in-plane magnetic field. Phys Rev B 1989, 40: 8508. 10.1103/PhysRevB.40.8508View ArticleGoogle Scholar
- Gavrila M, Kaminski JZ: Free-free transitions in intense high-frequency laser fields. Phys Rev Lett 1984, 52: 613. 10.1103/PhysRevLett.52.613View ArticleGoogle Scholar
- Pont M, Walet NR, Gavrila M, McCurdy CW: Dichotomy of the hydrogen atom in superintense, high-frequency laser fields. Phys Rev Lett 1988, 61: 939. 10.1103/PhysRevLett.61.939View ArticleGoogle Scholar
- Sari H, Kasapoglu E, Sökmen I: The effect of an intense laser field on magneto donors in semiconductors. Phys Lett A 2003, 311: 60. 10.1016/S0375-9601(03)00456-0View ArticleGoogle Scholar
- Kasapoglu E, Sari H, Güneş M, Sökmen I: Magnetic field and intense laser radiation effects on the interband trasnsitions in quentum well wires. Surface Rev Lett 2004, 11: 403. 10.1142/S0218625X04006335View ArticleGoogle Scholar
- Kasapoglu E, Sökmen I: The effects of intense laser field and electric field on intersubband absorption in a double-graded quantum well. Physica B 2008, 403: 3746. 10.1016/j.physb.2008.06.024View ArticleGoogle Scholar
- Diniz Neto OO, Qu F: Effects of an intense laser field radiation on the optical properties of semiconductor quantum wells. Superlatt Microstruct 2004, 35: 1. 10.1016/j.spmi.2004.05.004View ArticleGoogle Scholar
- Niculescu EC, Eseanu N: Interband absorption in square and semiparabolic near-surface quantum wells under intense laser field. Eur Phys J B 2011, 79: 313. 10.1140/epjb/e2010-10556-3View ArticleGoogle Scholar
- Eseanu N: Intense laser field effect on the interband absorption in differently shaped near-surface quantum wells. Phys Lett A 2011, 375: 1036. 10.1016/j.physleta.2010.12.077View ArticleGoogle Scholar
- Fox AM, Miller DAB, Livescu G, Cunningham JE, Jan WY: Excitonic effects in coupled quantum wells. Phys Rev B 1991, 44: 6231. 10.1103/PhysRevB.44.6231View ArticleGoogle Scholar
- Galbraith I, Duggan G: Exciton binding energy and external-field-induced blue shift in double quantum wells. Phys Rev B 1989, 40: 5515. 10.1103/PhysRevB.40.5515View ArticleGoogle Scholar
- Yu P, Cardona M: Fundamentals of Semiconductors, 3rd ed. Springer, Berlin; 2003.Google Scholar
- Sadowski J: Excitonic luminescence in strained quentum wells. Opto-Electr Rev 1996, 4: 135.Google Scholar
- Baser P, Elagoz S, Baraz N: Hydrogenic impurity states in zinc-blende InxGa1−xN/GaN in cylindrical quantum well wires under hydrostatic pressure. Physica E 2011, 44: 356. 10.1016/j.physe.2011.08.027View ArticleGoogle Scholar
- Duque CA, Mora-Ramos ME, Kasapoglu E, Sari H, Sökmen I: Combined effects of intense laser field and applied electric field on exciton states in GaAs quantum wells: transition from the single to double quantum well. Phys Stat Sol B 2012, 249: 118. 10.1002/pssb.201147250View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.